Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Synthesis and Characterization of Carbon Nanotube Supported Pt-Au Catalyst and Its Microwave Assisted N-Hexane Decomposition Measurements

Mohammed Ali Salih, Aykut Çaglar, Arif Kivrak, Hilal Kivrak*

Chemical Engineering Department, Van Yüzüncü Yıl University, Van, Turkey

Abstract: Herein, CNT supported Pt and Pt-Au catalysts were carefully synthesized via NaBH₄ reduction method. Pt-Au catalysts were obtained at varying ratios. For all of these CNT supported Pt and Pt-Au catalysts, BET, EDX, and XRD measurements were performed. The atomic ratio of the catalyst was obtained by EDX analysis. Surface area was defined via BET and crystal structure was examined by XRD. For microwave assisted n-hexane reforming measurements, microwave reactor was used to investigate the decomposition of n-hexane on CNT supported bimetallic Pt-Au catalysts. After applying microwave heating during the reaction time, the volume change is defined and read out. As a result, it was observed that Pt-Au catalysts prepared at 50:50 atomic ratio gives the best catalytic activity.

Keywords: Pt, Pt-Au, CNT, nanocatalyst, n-hexzane, decomposition, microwave assisted heating

Citation: Mohammed Ali Salih, Aykut Çaglar, Arif Kivrak, Hilal Kivrak, Synthesis and Characterization of Carbon Nanotube Supported Pt-Au Catalyst and Its Microwave Assisted N-Hexane Decomposition Measurements. Nanoscience and Nanotechnology Research, 4 (4). 132-134. January 2017. doi:10.12691/nnr-4-4-3

1. Introduction

Energy is important and permanent needs for human kind. Fossil fuels such as oil, coal and natural gas are the currentlu used fuels. Nevertheless, it is predicted that fossil fuel will exhaust n the near future. According to the Hubbert theory, the global production of fossil fuels will start to decrease by 2020 [1]. Thus, the researchers are intensively studying on the alternative energy sources [2,3,4,5,6,7] In that context, heterogeneous catalysis is also crucial for these studies to provides a promising means to develop alternative energy technologies. In this regard, catalysts having high activity and high selectivity should be produced [8].

Gasoline is a mixture of hydrocarbons. It could be used as a fuel in internal combustion engines (ICEs). Due to its high extent consumption in automobile industry, the request for the gasoline is increasing globally [9,10]. The catalytic reforming is an important process. During the catalytic eforming of n-hexane, naphtha was converted into high-octane reformates [11]. Hydrocarbons or naphtha have low octane number. Hence, it is not suitable to use them directly for direct gasoline blending. Therefore, catalytic reforming of naphtha and isomerization of light alkanes are required to enhance the gasoline quality (>70). High octane numbers relate to good engine performance [12] .

Heterogenous catalysts consisting of metal nanoparticles onto supports could be synthesized via various techniques. Furthermore, their catalytic activity could be investigated in a number of catalytic chemical reactions. One could note that activity could be enhanced greatly by varying the size, shape and composition of nanoparticle [13]. For instance, it was reported that when pure mesoporous silica (MCF-17) was modified with Aluminum, Lewis acid sites were created. This material is not active for the n hexane catalytic reforming. When it is modified with colloidally synthesized platinum nanoparticles, the catalyst showed enhanced activity [8,14,15]. Ni and Pt-Ni were also used to increase the ativity of catalytic reforming [12]. It was reported that the bimetallic catalysts presented a higher activity in the isomerization of n-hexane compared to the monometallic ones.

N-hexane decomposition is an important parameter for the n-hexzane catalytic reforming process. At present, ne-hexzane decomposition was examined on CNT supported Pt and Pt-Au bimetallic catalysts under microwave irradiation. In our previous, microwave irradiation was also used for different applications [16,17]. CNT supported Pt and Pt-Au catalysts were prepared by NaBH₄ reduction method, characterized via BET, EDX, and XRD.

2. Materials and Methods

2.1. Catalyst Preparation

In this research, the synthesis weight 0.1 g of Carbon Nano Tube (CNT) support dissolved in 40 ml water and stirrer for 10 min. Then, H₂Cl₆Pt₆.xH₂O precursor was added to the catalyst solution for absorbent CNT to Pt stay in ultrasonic bath about 20 min. Following this, the different amount of NaBH₄ was added to the solution for reduction after 20 min in ultrasonic As a result, the obtained precipitate was filtrated, washed with by-distilled water and dried at oven vacuum 75 °C. By this method, CNT supported Pt catalysts was obtained. The synthesis details of the CNT supported Pt catalysts were given Table 3.1. For the synthesis of CNT supported Pt-Au catalysts, 0.1 g of CNT support was used and dissolved in the water. Then, this mixture was ultrasonicated and stirred for 10 min and H₂Cl₆Pt₆.xH₂O precursor was dissolved in the same kind of solvent for absorbent CNT to Pt. These two solution were mixed, ultrasonicated and stirred for 20 min. Then NaBH₄ was added to reduce this solution and ultrasonicated for reduction after 20 min in ultrasonic bath. Following this, AuCl was added to this solution and further reduction was performed. A precipitate was obtained, filtrated, washed with by-distilled water and dried under 75 °C an oven vacuum. As a result, Pt-Au catalysts was obtained at varying ratios. The synthesis details of the CNT supported Pt-Au catalysts were given Table 1.

Table 1. Details of the preparation method on CNT supported Pt and Pt-Au catalysts prepared by NaBH₄ reduction method

2.2. Catalyst Characterization

The atomic ratio of the CNT supported Pt and Pt-Au catalysts was obtained by EDX analysis using a scanning electron microscope Phillips XL30 with a 20 keV electron beam. X-ray diffraction (XRD) analyses were performed using a Rigaku diffractometer model Miniflex II using Cu Kα radiation source. The diffractograms were recorded from 2θ = 50° to 85° with a step size of 0.05° and a scan time of 2 s per step. All the catalysts and the characterization methods used for these catalysts were given in Table 2.

Table 2. Details of the characterization methods on CNT supported Pt and Pt-Au catalysts

2.3. N-Hexzane Decomposition Measurements

In this study, a Microwave Anton Paar reactor was used to investigate the decomposition of n-hexane on CNT bimetallic catalysts. 0.05 g catalyst was inserted in 20 ml reactor tube. Furthermore, 10 ml n-hexane was added in to the reactor tube. Then, this mixture was heated to 150 °C and its temperature was kept constant at this temperature for 30 min. At the end of the 30 min, the tube was cooled and removed from the reactor. The volume change is defined and read out.

3. Results and Discussion

Characterization results of these catalysts were given on Table 3. The elemental compositions of these catalysts investigated using EDX spectroscopy were given in Table 3. Considering all CNT supported Pt and Pt-Au catalysts, the nominal weight percent of Pt is 10% and the EDX results show that weight percentage of Pt is around 10% similar to the nominal values. Furthermore, BET surface areas were also given on Table 3. According to these values, BET surface areas decrease by increasing metal loading.

Table 3. Characterization results on CNT supported Pt and Pt-Au catalysts

X-ray diffractograms of Pt-Au (50:50) catalyst were given in Figure 1. XRD pattern of this catalyst exhibited a broad peak at about 2θ = 25° associated to the carbon support material. Furthermore, (111), (200), (220) of face centered cubic (fcc) structure of Pt and Pt alloys were presented at XRD pattern.

Figure 1. XRD patterns of CNT supported Pt-Au (50:50) catalysts

N hexane decomposition measurements were performed on Pt and Pt-Au catalysts. The volume change was given for every catalyst on the Table 4. It was observed that Pt-Au catalysts at prepared at 50:50 atomic ratio gives the best catalytic activity.

Table 4. N hexane decomposition results on CNT supported Pt and Pt-Au catalysts

4. Conclusions

In the light of the experimental results, the following conclusion could be drawn:

• CNT supported Pt and Pt-Au catalysts at different atomic ratios were prepared succesfully via NaHB₄ reduction method

• Pt and Pt-Au catalysts were characterized by BET, EDX, and XRD.

• EDX measurements revealed that catalysts were prepared at the desired Pt content.

• BET measurements indicated that Au addition leads to decrease the surface area of bimetallic catalysts.

• XRD pattern of Pt-Au catalyst indicate Pt fcc peaks belonging the Pt-Au structure were observed.

• Best catalytic activity for the n-hexzane decomposition reaction was obtained for Pt-Au (50:50)/CNT catalyst.

Acknowledgements

Authors would like to thank for the financial support for The Scientific and Technological Research Council of Turkey (TUBITAK) project (project no: 113Z249) and TUBITAK project (Project no: 114M156).

References

[1]   | Barton, J. and R. Gammon, The production of hydrogen fuel from renewable sources and its role in grid operations. Journal of Power Sources, 2010. 195(24): p. 8222-8235.
[2]   | Tümay, M., et al., A review of magnetically controlled shunt reactor for power quality improvement with renewable energy applications. Renewable and Sustainable Energy Reviews, 2017. 77: p. 215-228.
[3]   | Sultana, W.R., et al., A review on state of art development of model predictive control for renewable energy applications. Renewable and Sustainable Energy Reviews, 2017. 76: p. 391-406.
[4]   | Berk, I. and V.Ş. Ediger, Forecasting the coal production: Hubbert curve application on Turkey's lignite fields. Resources Policy, 2016. 50: p. 193-203.
[5]   | Chavez-Rodriguez, M.F., A. Szklo, and A.F.P. de Lucena, Analysis of past and future oil production in Peru under a Hubbert approach. Energy Policy, 2015. 77: p. 140-151.
[6]   | Reynolds, D.B., World oil production trend: Comparing Hubbert multi-cycle curves. Ecological Economics, 2014. 98: p. 62-71.
[7]   | Anderson, K.B. and J.A. Conder, Discussion of Multicyclic Hubbert Modeling as a Method for Forecasting Future Petroleum Production. Energy & Fuels, 2011. 25(4): p. 1578-1584.
[8]   | Somorjai, G.A. and Y. Li, Introduction to surface chemistry and catalysis. 2010: John Wiley & Sons.
[9]   | Awad, O.I., et al., Using fusel oil as a blend in gasoline to improve SI engine efficiencies: A comprehensive review. Renewable and Sustainable Energy Reviews, 2017. 69: p. 1232-1242.
[10]   | Gentner, D.R., et al., Review of Urban Secondary Organic Aerosol Formation from Gasoline and Diesel Motor Vehicle Emissions. Environmental Science & Technology, 2017. 51(3): p. 1074-1093.
[11]   | An, K., et al., High-Temperature Catalytic Reforming of n-Hexane over Supported and Core–Shell Pt Nanoparticle Catalysts: Role of Oxide–Metal Interface and Thermal Stability. Nano Letters, 2014. 14(8): p. 4907-4912.
[12]   | Martins, G.S., et al., n-Hexane isomerization on Ni-Pt/catalysts supported on mordenite. Modern Research in Catalysis, 2013. 2(04): p. 119.
[13]   | Musselwhite, N., et al., Isomerization of n-Hexane Catalyzed by Supported Monodisperse PtRh Bimetallic Nanoparticles. Catalysis Letters, 2013. 143(9): p. 907-911.
[14]   | An, K., et al., Designed Catalysts from Pt Nanoparticles Supported on Macroporous Oxides for Selective Isomerization of n-Hexane. Journal of the American Chemical Society, 2014. 136(19): p. 6830-6833.
[15]   | Alayoglu, S., et al., Reforming of C-6 hydrocarbons over model Pt nanoparticle catalysts. Topics in catalysis., 2012. 55(11-13): p. 723-730.
[16]   | Sahin, O., et al., Facile and Rapid Synthesis of Microwave Assisted Pd Nanoparticles as Non-Enzymatic Hydrogen Peroxide Sensor. Int. J. Electrochem. Sci, 2017. 12: p. 762-769.
[17]   | Kivrak, H., O. Alal, and D. Atbas, Efficient and rapid microwave-assisted route to synthesize Pt–MnOx hydrogen peroxide sensor. Electrochimica Acta, 2015. 176: p. 497-503.